1 STAR 193 RLS Bonded Cement Based Material Overlays for the Repair, the Lining or the Strengthening of Slabs or Pavements This publication has been published by Springer in 2011, ISBN This STAR report is available at the following address: Please note that the following PDF file, offered by RILEM, is only a final draft approved by the Technical Committee members and the editors. No correction has been done to this final draft which is thus crossed out with the mention "Unedited version" as requested by Springer.
2 TABLE OF CONTENT 1. INTRODUCTION (J.-L. Granju, B. Bissonnette, L. Courard) 2. OVERLAY DESIGN PROCESS (D.W. Fowler, M. Treviño) Abstract 2.1 Purpose of overlays 2.2 Materials selection Slabs on grade/pavements Concrete Reinforcement Structural slabs and decks Concrete Reinforcement 2.3 Joints Slabs on grade/pavements Structural slabs and decks 2.4 Construction procedures Steel placement Environmental effects Curing 2.5 The BCO process Project selection Design Construction Quality control/quality assurance (QA/QC) 2.6 Conclusions References 3. CONDITION EVALUATION OF THE EXISTING STRUCTURE PRIOR TO OVERLAY (L. Courard, M. Treviño, B. Bissonnette) Abstract 3.1 Introduction 3.2 Assessment of pavement/substrate base Principles of evaluation Condition survey of distress Visual examination Structural investigations Interpretation Test methods for pavement/substrate base Deflection testing Modulus of elasticity
3 Subgrade modulus Concrete flexural strength Load transfer efficiency (LTE) 3.3 Assessment of structural slab/deck/support Introduction Condition survey of distress Structural evaluation Material evaluation Test methods and procedures Non destructive testing for the estimation of strength Schmidt rebound hammer Ultrasonic Pulse Velocity (UP V) Probe penetration Pull out test Break off test Pull off test Optic fibres Non destructive tests for flaw detection and condition assessment Stress wave propagation methods Infrared thermography Ground penetrating radar (GPR) Electrical and magnetic methods for reinforcement Nuclear (radioactive) methods Methods for the determination of superficial porosity Principles Capillary suction coefficient Mercury intrusion porosimetry In situ tests Methods for the determination chemical damages 3.4 Feasibility analysis References 4. BOND (J. Silfwerbrand, H. Beushausen, L. Courard) Abstract 4.1 Classification of bond 4.2 Definition of bond strength 4.3 Fundamental bond mechanisms 4.4 Factors affecting bond Concrete properties Fresh material properties Hardened material properties Overlay strength Removal of deteriorated concrete Concrete removal behind rebars, rebar cleaning, and rebar replacement Cleaning after concrete removal Surface properties Surface preparation
4 4.4.7 Bonding agents Mechanical devices crossing the interface Concrete placement Concrete curing Short-term bond properties Long-term bond properties Traffic vibrations 4.5 Test methods General Shear test methods Comparisons between tensile bond strength and shear bond strength 4.6 Evaluation 4.7 Design strength values 4.8 Performance requirements References 5. STRUCTURAL BEHAVIOUR (E. Denarié, J. Silfwerbrand, H. Beushausen) Abstract 5.1 Introduction 5.2 Actions 5.3 Performance of composite structures 5.4 Different forms of restraint and effect of joints 5.5 Mechanical behaviour of composite structures with cementitious materials of different ages Overview of existing analytical models Normal stresses due to differential shrinkage in composite beams with complete bond Shear stresses due to differential shrinkage in composite beams Normal and shear stresses due to differential shrinkage in composite beams with incomplete bond 5.6 Experimental tests Swedish tests on mechanically loaded concrete beams Swedish tests on concrete beams subjected to differential shrinkage Swedish tests on concrete slabs Tests at EPFL on composite beams with normal concretes of different ages Other tests 5.7 On restrained shrinkage set-ups 5.8 Numerical modelling 5.9 Conclusions 5.10 Outlook for future research References
5 6. DEBONDING (A. Turatsinze, H. Beushausen, R. Gagné, J.-L. Granju, J. Silfwerbrand, R. Walter) Abstract 6.1 Introduction 6.2 Impact of debonding 6.3 Brief summary of debonding 6.4 Methods for monitoring debonding Non destructive methods Semi destructive methods Laboratory tests 6.5 Debonding mechanism 6.6 Debonding modeling 6.7 Role of reinforcement of overlays In situ findings Need to distinguish between first monotonic loading and shrinkage-precracking plus fatigue First monotonic loading Shrinkage pre-cracking and fatigue loading Conclusion 6.8 Crack propagation and crack opening First monotonic loading Shrinkage-pre-cracking and fatigue loading 6.9 Special overlays Stang and Walter s results Anchoring of the overlay 6.10 Boundaries and joints of the overlays Boundaries and full depth joints Sawn joints 6.11 Conclusion References 7. DESIGN (M. Treviño, j.-l. Granju, h. Beushausen, a. Chabot, h. Mihashi, j. Silfwerbrand) Abstract 7.1 Introduction 7.2 Design for sufficient strength Overview Purpose of the overlay Basic design principle Design concepts Overall standard deviation
6 7.2.3 Current overlay design procedures Corps of Engineers Portland Cement Association AASHTO Reinforcement design of overlaid continuously reinforced concrete pavements (CRCP) BCO design procedures in other countries Summary and conclusions 7. 3 Design to prevent debonding Introduction USA recommendations European requirements Japanese requirements Swedish practice Expected design shear strength 7.4 Conclusion References 8. PRACTICE AND QUALITY ASSURANCE (M. Vaysburd, B. Bissonnette, R. Morin) Abstract 8.1 Scope and definitions 8.2 Importance of substrate surface preparation General Safety 8.3 Concrete removal General Removal methods Advantages and limitations of concrete removal methods Basic methods Combining methods 8.4 Substrate surface preparation General Pre-overlay repairs Surface General Concrete surface cleaning Reinforcement cleaning, inspection and repair Moisture conditioning of the substrate prior to overlay/repair General Optimum water condition of the substrate Maintenance of the prepared substrate Quality control of surface preparation Test repair Required strength at the interface 8.5 Application
7 8.5.1 General Workmanship Basic requirement Repair placement Consolidation Surface finishing Curing 8.6 Quality assurance / construction inspection Scarification and removal of unsound concrete Substrate preparation Placement and consolidation References 9. MAINTENANCE AND REPAIR OF OVERLAYS (D.W. Fowler) Abstract 9.1 Types and causes of distress 9.2 Evaluation of damage 9.3 Repair methods Cracks Delaminated concrete Spalls 9.4 Conclusions 10. CONCLUSION (B. Bissonnette, L. Courard, J.-L. Granju)
8 TC 193-RLS: Bonded cement-based material overlays for the repair, the lining or the strengthening of slabs or pavements Réparation, re-surfaçage ou renforcement des dallages industriels ou des chaussées par un rechargement adhérent à base cimentaire Membership Name Organization Country Status B. Bissonnette CRIB - Université Laval (Québec, QC) Canada Chairman H. Beuschausen University of Cape Town (Cape Town) South Africa Member A. Chabot LCPC Nantes (Nantes) France Associate L. Courard Université de Liège (Liège) Belgium Secretary L. Czarnecki Warsaw University of Technology (Warsaw) Poland Member E. Dénarié EPFL Lausanne (Lausanne) Switzerland Member R. Gagné University of Sherbrooke (Sherbrooke, QC) Canada Associate A. Garbacz Warsaw University of Technology (Warsaw) Poland Member J.-L. Granju LMDC INSA Toulouse (Toulouse) France Honorary chair D.W. Fowler University of Texas (Austin, TX) U.S.A. Member H. Mihashi Tohoku University (Sendai) Japan Associate R. Morin Ville de Montréal (Montréal, QC) Canada Member A. Müller CRIB - Université Laval (Québec, QC) Canada Member J. Silfwerbrand Swedish C&C Research Inst. (Stockholm) Sweden Member M. Treviño Center for Transportation Research, University of Texas (Austin, TX) U.S.A. Associate A. Turatsinze LMDC INSA Toulouse (Toulouse) France Member A.M. Vaysburd Vaycon Consulting (Baltimore, MD) U.S.A. Member R. Walter Technical University of Denmark (Lyngby) Denmark Associate
9 1. INTRODUCTION J.-L. Granju (1), B. Bissonnette (2), L. Courard (3) (1) Laboratoire Matériaux et Durabilité des Constructions (LMDC), UPS-INSA, Toulouse, France (2) Centre de Recherche sur les Infrastructures en Béton (CRIB), Université Laval, Québec (QC), Canada (3) GeMMe Building Materials, ArGEnCo Department, University of Liège, Belgium 1.1 INTRODUCTION Concrete has been used in construction for more than a century now and a number of existing structures exhibit distresses and/or lack of load carrying capacity. Repair and strengthening of existing structures are in fact among the biggest challenges civil engineers will have to face in the years to come. Moreover, the number of concrete structures keeps growing, and therefore repair or retrofitting needs keep increasing. Present concerns of sustainable development emphasizing rehabilitation instead of new construction, acts as incentive to this trend. Among different approaches that can be considered for concrete rehabilitation, bonded overlays are often the most economical alternative. Overlays are particularly suitable in the case of structures with large surface areas, where it can be either poured or sprayed. The following types of applications are of special concern: slabs on grade (for example, industrial floors), pavements, bridge decks, walls and tunnels. Toppings and linings are also relevant to the same type of problem. The primary purpose of overlays is to extend the life of the candidate concrete structures, either by restoring a smooth sound surface and/or the original load carrying capacity, or by improving the load carrying capacity by a thickness increase. For a slab or pavement in good condition, a 25 % increase in thickness can nearly double its stiffness in some cases, resulting in nearly a 50 % reduction in flexural stress and a significant increase of its service life. Other reasons for overlaying slabs or concrete pavements include: matching the level of an adjacent slab or element; replacing deteriorated or contaminated concrete and reinstating the protection of the structure (especially its reinforcement); providing a more durable wearing surface; improving the frictional characteristics of the surface for pavements or bridge decks; restoring architectural features such as colour or texture.
10 The potential for overlay applications worldwide sums up to multi millions of square meters. Nevertheless, the durability of bonded overlay systems still draw concerns in the technical community because of bond sustainability problems encountered in a number of cases. In such events, debonding is generally initiated at the boundaries, joints and cracks in the overlay, and can be aggravated by curling effects in the debonding area. That leads to new cracks and increased debonding, which accelerate the damage process and soon leads to the need of renewed repairs. At this time, there is still no accepted design approach or methodology that can warrant the practitioner a successful outcome of the repair. The available information essentially consists of quite general recommendations relying on experience and very simplistic design considerations. In order to progress through understanding and knowledge, the 193 RLS RILEM Technical Committee was created. Its goal was to set the basis for the development of relevant design rules and technical recommendations for the achievement of durable bonded overlays (for repair or strengthening). The primary concern in the scope of work of this TC is the "bond" between the overlay and the repaired structure (the latter is often referred to as the substrate). Indeed, it is the foremost factor in a bonded overlay system, provided that a durable repair material is used and that the residual concrete base is sound, and its durability is synonymous of durability of the whole composite system. A rational and reliable design requires a thorough understanding of the bond and debonding mechanisms. The quality of the bond depends on both the substrate preparation and the overlay placement procedure. In this respect, the quality of workmanship is of major importance. Debonding generally results from a combination of internal stresses induced by the gravity loads and the differential drying and thermal length changes between the overlay and the substrate. Irrespective of the source of internal stresses, the same mechanism governs debonding initiation and propagation. Two main overlay families must be distinguished: on the one hand, the bridge deck overlays and, on the other hand, the overlays performed on slabs on ground or on pavements. This State of the Art document is the major deliverable of 193 RLS TC. It is intended to provide a wide and accurate survey of current knowledge and practice, such as to identify rationally what is really understood, what the shortcomings are, and from that on, what information needs to be generated to progress towards a real overlay design process. A subsequent task of the members of this TC will be the writing of Recommendations for reliable and durable repairs, which will be published in a separate document. In addition, the State of the Art report highlights inconsistencies in the terminology and definitions found in the scientific documentation, depending on the country, the sector of the industry, etc. The Recommendations document will propose some clarifications, based upon the consensus reached among the TC members.
11 This State of the Art report is divided into ten chapters. Chapter 1: Introduction. Chapter 2: Overlay: decision and construction process. This chapter first reports, through flow charts, a typical decision process methodology. Then a review of all relevant aspects of design and construction is proposed: material selection for the overlay, reinforcement considerations if applicable (rebars, fibre reinforcement), interface with the substrate, joints, environmental effects, curing of the overlay, and quality assurance/quality control. Throughout this review, distinctions are made between the main types of overlay applications (slabs or pavements and bridge decks). Chapter 3: Condition evaluation of the existing structure prior to overlay. The first part of this chapter presents a guide to assess the condition of the substrate and to determine whether a bonded overlay is a relevant solution for the structure under evaluation. The second part provides a survey and detailed description of available test methods for condition evaluation of concrete structures. Chapter 4: Bond. This chapter first presents an exhaustive overview of all the factors affecting the bond (favorably or unfavorably), from surface preparation to the use of bonding agents. The available testing procedures for bond characterization are then discussed. Finally, the existing recommendations to yield a durable bond are summarized. Chapter 5: Structural behavior. This chapter deals with the structural behavior of a composite system made of an existing substrate and a bonded cement based overlay. Through a review of analytical models, the mechanical response of the repair composite is addressed, taking into account gravity loads, thermal and hygrometric strains, material ageing, as well as boundary conditions such as the degree of restraint and the presence of joints. Special attention is paid to restrained deformations, inherent to repaired concrete members. Then, an overview of relevant experimental work and numerical modeling is presented. Chapter 6: Debonding. In this chapter, emphasis is put on debonding, which can lead to the failure of an overlaid system through partial or total loss of composite action. A summary of field observations and a survey of existing test methods to detect debonding are first proposed. Debonding mechanisms are then described, from initiation to propagation, as a result of length changes and/or repeated gravity loads (fatigue). Further on, proposed modeling approaches are discussed. Supported by experimental data, modeling is used to demonstrate and help understanding the benefits of different reinforcement/anchoring solutions. Finally, the influence of joints in an overlaid structure is reviewed. Chapter 7: Design.
12 This chapter summarizes the existing design rules, recommendations and requirements for bonded concrete overlays, as found in the guidelines of some of the foremost organizations around the world. The proposed approaches go from very simplistic criteria, such as minimum bond strength or stress level limitations, to slightly more sophisticated design methods. Chapter 8: Practice and Quality Assurance. This chapter sums up the fundamentals of current good field practice, from substrate preparation to placement and curing of the overlay. It is completed with recommendations for proper quality control and quality assurance. Chapter 9: Maintenance and repair of overlays. Although bonded overlays are an attractive and improving repair alternative, they still carry some uncertainty and, sometimes, unsuccessful repairs have to be dealt with. This chapter describes the suitable repair methods or techniques. Chapter 10: Conclusion.
13 2. OVERLAY DESIGN PROCESS D.W. Fowler (1) and M. Treviño (2) (1) The University of Texas at Austin (TX), U.S.A. (2) Center for Transportation Research, The University of Texas at Austin, U.S.A. ABSTRACT Bonded concrete overlays have been used for nearly 100 year to extend the life of pavements, concrete slabs, bridge decks or other structural slabs. First, this chapter describes material selection, for slabs on grade and pavements; joints; and construction procedures including steel placement, environmental effects, and curing. Secondly, the bonded concrete overlay (BCO) process is described: the steps required in project selection; design of the BCO; construction, and quality assurance with flow charts included to provide a graphical overview. 2.1 PURPOSE OF OVERLAYS Bonded concrete overlays (BCO s) have been used since The primary purpose of overlays is to extend the life of a concrete slab or pavement, bridge deck or other structural slab. It has been shown [1, 2] that as the remaining life of a pavement decreases due to distress, e.g. cracking, spalling or punchouts, the life can be extended significantly by the use of a bonded concrete overlay. For a slab or pavement in good condition, a 25 % increase in thickness can nearly double the stiffness, resulting in nearly a 50 % reduction in flexural stress. Other reasons for overlaying concrete pavements or slabs include: provide an improved frictional surface for pavements or bridges; provide a smooth surface for industrial floors or buildings;
14 increase the elevation of the top surface to match an adjacent slab; provide a more durable wearing surface; repair corrosion damaged slabs or bridge decks with sound, durable concrete; and provide architectural features such as color or texture. 2.2 MATERIALS SELECTION Slabs on grade/pavements Concrete The cement content of the BCO concrete must be high enough to ensure that the available paste is sufficient to achieve bond at the interface, which eliminates the need for a bonding agent, and to meet strength and permeability requirements. Reduced paste requirements may be met by using well graded aggregates. Some specifications mandate minimum cement content, e.g. 390 kg/m 3 for normal overlay concrete and 490 kg/m 3 for dense overlay concrete. Lower levels of cement are desirable to reduce cost, reduce heat of hydration and reduce shrinkage. Reduced cost and reduced heat of hydration may also be accomplished by using fly ash as cement replacement; the addition of fly ash also has the advantages of improving durability and, in many cases, ultimate strength. The water cement ratio is determined by strength and durability (permeability) requirements. Generally, a water cement ratio of 0.40 will provide good durability and strength. One specification requires a water cement ratio of 0.40 for normal overlay concrete and 0.32 for dense overlay concrete. Aggregates should be selected for workability; aggregates should also have adequate durability for the intended application. The paste requirement may be reduced by improving overall aggregate gradation as suggested by Shilstone [3, 4] and Crouch . Shilstone suggests incorporating an intermediate aggregate, and this may be particularly helpful when using steel fibers. Admixtures will often include air entraining agent, which will help workability and improve freezing and thawing resistance. The use of fly ash may require greater dosages of air entraining agent to achieve the same percentage of entrained air. High range water reducers are often specified, and the amount should be based on trial batches. The addition or retarders in hot weather helps to preserve workability until the concrete can be placed and finished without affecting strength development Reinforcement Steel reinforcing and steel and synthetic fibers have been used as reinforcement. Steel reinforcing has been used in the form of tied bars and welded mats. Steel fibers have been used successfully in overlays to control cracks and to minimize drying shrinkage cracking. Normal steel fiber contents for steel fiber reinforced concrete are normally in the range of 1 to 2 % by volume. The amount of fibers required to achieve the desired result will depend on the type of fiber based on its bond characteristics.
15 Synthetic fibers should be used at a minimum of 0.25 % by volume; however, significant benefits have been obtained by using up to 1 % volume Structural slabs and decks Concrete Overlays for structural slabs and decks are generally used to replace removed concrete since the slab or deck cannot tolerate additional dead load and still continue to carry the design live load. One of the main applications of overlays for structural slabs is to replace deteriorated concrete due to corrosion of the steel reinforcing. The original concrete is removed to a depth of about 25 mm below the steel, and the overlay is used to reinstate the original surface. Generally, very durable, low permeability concrete is specified. Guidelines similar to those outlined for pavements are appropriate for structural slabs. In addition, latex, e.g. styrene butadiene, is often added (15 % latex solids by weight of cement) to provide improved bonding, greater flexural strength and decreased permeability Reinforcement Steel bars are normally used for structural slabs and decks. Often the original bars are adequate, although if significant reduction in cross section due to corrosion has occurred, the affected bars should be spliced with adequate anchorage length or replaced. In some cases when extensive replacement of reinforcing is required, corrosion resistant bars, e.g. epoxy coated steel, galvanized, or stainless steel may be considered for use in highly corrosive environments. Fibers, steel or synthetic, may be used for crack control and to minimize shrinkage cracking. 2.3 JOINTS Slabs on grade/pavements Jointed slabs and pavements usually require that the joints in the original slab or pavement be reinstated which is time consuming and costly. Sawing the joints and applying suitable high elongation joint filler is one possible solution. In some cases it may be possible to clean the joints of debris and apply joint filler. If it essential to reinstate the dowels at joints to prevent faulting, precast joint units have been used by removing the concrete for approximately 600 mm on each side of the joint and installing the units which have dowels in place. The overlays must be constructed to maintain the integrity of the joints. Saw cutting followed by application of suitable high elongation joint filler may be the optimum solution Structural slabs and decks Joints in structural slabs and decks are expansion joints. In some cases the nosings at the joints of the original concrete have spalled and deteriorated and must be repaired. The concrete in the overlay at the joints must have the durability and toughness to resist the impact of vehicular traffic,
16 where applicable, and one solution is to use very strong, impact resistant concrete headers on either side of the joints to which the overlay can be butted. 2.4 CONSTRUCTION PROCEDURES Steel placement Research has shown that the reinforcing placed on the substrate of a 75 mm thick slab with a 75 mm overlay cast on the surface will achieve the same pull out bond strength as reinforcing placed at mid depth of a 150 mm thick slab; all bars failed in tension . Placing the reinforcing on the substrate saves construction time and labor Environmental effects Weather conditions during construction of the overlay can be critical. Hot, dry climates cause the most problems because of the excessive evaporation of water from the concrete that often results. High evaporation rates during placements can result in plastic shrinkage cracking. Evaporation rate is a function of wind velocity, relative humidity, concrete temperature, and air temperature. An evaporation rate of 1 kg/m 2 or higher has been suggested as sufficiently high to cause plastic shrinkage cracking, but even lower values may cause problems. The evaporation rate can be estimated from published monographs [7, 8] or calculated from the equation. The evaporation rate should be monitored through construction by the use of a weather station which measures the four factors that influence evaporation. If the threshold value of evaporation rate is approached, action should be taken: discontinue placement of the overlay or provide measures to reduce evaporation including improved curing methods. Concrete temperature should be monitored throughout construction. Temperature at placement has been shown to have a significant effect on performance . Pavements placed in high temperatures in the summer have been found to have poor performance based on such indicators as crack spacing and distress occurrence compared to pavements placed in cooler weather. Therefore, for best performance the BCO placement temperature should be kept relatively low to avoid high temperatures of hydration. The surface of the substrate should not be permitted to exceed a temperature of 50 C . Another environmental issue that can be detrimental to the concrete performance is the temperature differential that occurs in the hours following placement. High ambient temperature differentials within 24 hours after placement may cause extensive thermal cracking; drops in temperature from the peak high temperature to the low temperature should not exceed 15 C . The largest drops in temperature in the concrete are usually associated with concrete placements in the morning in hot weather, which leads to the maximum hydration temperature occurring in combination with the maximum ambient temperature in the afternoon, followed by a large reduction in ambient temperature during the night. The rapid cooling of the surface can lead to thermal contraction strains that exceed the capacity of the concrete at that young age. Weather forecasts should be consulted to determine if placement conditions will be likely to cause problems.
17 If any of the adverse environmental conditions described in this section occurs during the placement of the concrete, placement should be avoided unless the conditions can be offset by such measures as: cooling the aggregates or concrete; special curing methods discussed in a following section; or use of fly ash as cement replacement to lower the heat of hydration Curing Proper curing procedures are necessary to avoid excessive moisture loss at early ages that can result in plastic shrinkage and loss in tensile strength capacity at the surface. Curing should begin as soon after placement and finishing as possible to minimize loss of bleed water. Curing may be accomplished by: 1) Application of curing compound. For textured or tined surfaces the spray application should be applied from two directions to ensure that the entire surface is coated. 2) Application of membrane curing. Various liquid sealing compounds, e.g. bituminous and paraffinic emulsions, coal tar cut backs, pigmented and non pigmented resin suspensions, or suspensions of wax or non liquid protective coating such as sheet plastics or waterproof paper, are used to restrict evaporation of water. 3) Curing blankets. A covering of sacks, mattings, burlap, straw, or other suitable paper is placed over the surface to reduce evaporation and to reduce the temperature reduction at the surface. When used to reduce evaporation the blankets are generally wetted. 4) Monomolecular film. Monomolecular films (MMF) are compounds that form a thin monomolecular film to reduce rapid moisture loss from the concrete surface prior to curing. Another curing method should be used after the evaporation retardant is sprayed on. Research has shown, however, that the use of MMF followed by application of curing compound does not consistently provide less evaporation than curing compound alone. Table 2.1 summarizes recommended curing procedures for bonded concrete overlays.
18 Table 2.1: Recommended curing for bonded concrete overlays Condition Evaporation below 0.5 kg/m 2 /hr Evaporation above 0.5 kg/m 2 /hr but below 1 kg/m 2 /hr Evaporation over 1 kg/m 2 /hr Temperature drop in next 24 hours less than 15 C below temperature at time of paving Temperature drop in next 24 hours more than 15 C below temperature at time of paving Recommendation Membrane curing Membrane curing, plus evaporation retardant or fogging or wet mats, in place for 12 hours Membrane curing, plus wet mat curing or fogging or other approved methods, in place 36 hours Membrane curing Membrane curing plus wet mats for 36 hours, or other approved methods 2.5 THE BCO PROCESS The BCO process is summarized in the flow chart in Fig Each step of the process will be discussed. Figure 2.1: BCO development process
19 2.5.1 Project selection The project selection involves several decisions as shown in the flow chart in Fig Figure 2.2: Flowchart of the project selection stage
20 Figure 2.2 (cont.): Flowchart of the project selection stage 1) Need for rehabilitation, which is based on level of deterioration, age and increase in traffic loadings. 2) Availability of resources to the owner/agency with the responsibility for maintaining the highway. 3) Type of rehabilitation: overlay versus non overlay. 4) Type of overlay if an overlay is selected. The overlay choices are portland cement concrete (PCC) and asphalt concrete. For PCC overlays the choice is between bonded and unbonded. 5) Timing and condition. A PCC overlay should be applied after structural failures have occurred but prior to functional failures at which time the pavement has reached a minimal level of serviceability. Figure 2.3 shows the pavement serviceability index (PSI) as a function of time and a hypothetical time at which structural failure and functional failure occurs. Once the decision is made to construct a BCO, the next step is the design.